Xianyu Liu 1, Liwen Ma 2, Yehong Du 2, Qiongqiong Lu 3,* , Aikai Yang 4 and Xinyu Wang 2,*
1 School of Chemistry and Chemical Engineering, Lanzhou City University, Lanzhou 730070, China; [email protected] 2 Institute of Materials and Technology, Dalian Maritime University, Dalian 116026, China; [email protected] (L.M.); [email protected] (Y.D.) 3 Leibniz Institute for Solid State and Materials Research (IFW) Dresden e.V., Helmholtzstraße 20, 01069 Dresden, Germany 4 Forschungszentrum Jülich GmbH, Institute of Energy and Climate Research, Materials Synthesis and Processing (IEK-1), 52425 Jülich, Germany; [email protected] * Correspondence: [email protected] (Q.L.); [email protected] (X.W.)
Abstract: Aqueous zinc-ion batteries (ZIBs) with the characteristics of low production costs and good safety have been regarded as ideal candidates for large-scale energy storage applications. However, the nonconductive and non-redox active polymer used as the binder in the traditional preparation of electrodes hinders the exposure of active sites and limits the diffusion of ions, compromising the energy density of the electrode in ZIBs. Herein, we fabricated vanadium pentoxide nanoﬁbers/carbon nanotubes (V O /CNTs) hybrid ﬁlms as binder-free cathodes for ZIBs. High ionic conductivity and 2 5 electronic conductivity were enabled in the V2O5/CNTs ﬁlm due to the porous structure of the ﬁlm Citation: Liu, X.; Ma, L.; Du, Y.; Lu, and the introduction of carbon nanotubes with high electronic conductivity. As a result, the batteries Q.; Yang, A.; Wang, X. Vanadium −1 −1 based on the V2O5/CNTs ﬁlm exhibited a higher capacity of 390 mAh g at 1 A g , as compared Pentoxide Nanoﬁbers/Carbon −1 −1 to batteries based on V2O5 (263 mAh g ). Even at 5 A g , the battery based on the V2O5/CNTs Nanotubes Hybrid Film for ﬁlm maintained a capacity of 250 mAh g−1 after 2000 cycles with a capacity retention of 94%. In High-Performance Aqueous Zinc-Ion −1 addition, the V2O5/CNTs ﬁlm electrode also showed a high energy/power density (e.g., 67 kW kg / Batteries. Nanomaterials 2021, 11, 1054. 267 Wh kg−1). The capacitance response and rapid diffusion coefﬁcient of Zn2+ (~10−8 cm−2 s−1) https://doi.org/10.3390/ nano11041054 can explain the excellent rate capability of V2O5/CNTs. The vanadium pentoxide nanoﬁbers/carbon nanotubes hybrid ﬁlm as binder-free cathodes showed a high capability and a stable cyclability,
Academic Editor: Giuseppe demonstrating that it is highly promising for large-scale energy storage applications. Cappelletti Keywords: aqueous zinc-ion battery; vanadium pentoxide; carbon nanotubes; hybrid ﬁlm Received: 19 March 2021 Accepted: 16 April 2021 Published: 20 April 2021 1. Introduction Publisher’s Note: MDPI stays neutral The lithium-ion battery is widely used in daily life owing to its many advantages with regard to jurisdictional claims in including a high operating voltage, high speciﬁc capacity, and long cycle life [1,2]. However, published maps and institutional afﬁl- lithium resources on the earth are limited, and the contradiction between its high price and iations. increasing demand is becoming increasingly prominent. In addition, lithium-ion batteries suffer other issues such as high internal resistance, harmful organic electrolytes, and safety hazards [3,4]. These problems restrict their large-scale applications. Rechargeable aqueous batteries have the merits of low production costs, and the electrolyte used is an aqueous Copyright: © 2021 by the authors. electrolyte with high safety. Therefore, it is expected to supplement lithium-ion batteries Licensee MDPI, Basel, Switzerland. for new-generation electrochemical energy storage systems [5–8]. This article is an open access article Among rechargeable aqueous batteries, aqueous zinc-ion batteries (ZIBs) have at- distributed under the terms and tracted more attention due to the high abundance of metal zinc in the earth’s resources, conditions of the Creative Commons low cost, and nontoxicity [9,10]. As zinc metal foil can be directly used as the anode, the Attribution (CC BY) license (https:// development of cathodes of ZIBs have become a research hotspot. The reported cathode creativecommons.org/licenses/by/ materials for ZIBs mainly include manganese compounds, vanadium oxides, Prussian blue, 4.0/).
Nanomaterials 2021, 11, 1054. https://doi.org/10.3390/nano11041054 https://www.mdpi.com/journal/nanomaterials Nanomaterials 2021, 11, 1054 2 of 10
and organic compounds [11–14]. Among these cathode materials, vanadium pentoxide 3+ 5+ (V2O5) has a unique layered structure with a wide range of valence states (from V to V ), which is conducive to the multielectron transfer providing a high speciﬁc capacity [15,16]. However, its ion conductivity is low and its diffusion kinetics is slow, resulting in a poor rate performance and unsatisﬁed cycle performance. Furthermore, the nonconductive and non-redox active polymer was used as the binder in the traditional preparation of electrodes, which hinders the diffusion of zinc ions and compromises the energy density of the electrode . Therefore, in order to avoid using binders, it is important to design a binder-free V2O5 electrode. In this work, V2O5 nanoﬁbers/carbon nanotubes (V2O5/CNTs) hybrid ﬁlms were fabricated and employed as the cathode of ZIBs, and the usage of nonconductive and non- redox active binders was avoided. The network structure of V2O5/CNTs ﬁlm is helpful for improving the electronic and ionic conductivity of the electrode. Compared with batteries with binders, the batteries based on the V2O5/CNTs ﬁlm showed a higher speciﬁc capacity and a better cycle stability. This work proved that the electrochemical performance of ZIBs can be improved by the application of binder-free electrodes.
2. Materials and Methods 2.1. Preparation of V2O5 Nanoﬁbers
First, 0.75 g of NH4VO3 (99%, Aladdin) and 1.25 g of P123 (Sigma-Aldrich, St. Louis, MO, USA) were dissolved in 75 mL of water containing 3.75 mL of 2 M of HCl. The mixture was stirred at room temperature for 7 h and then transferred into a Teﬂon autoclave. After the autoclave was sealed, it was held at 120 ◦C for 24 h and then cooled to room temperature. The product was washed with deionized water several times and then freeze-dried to obtain V2O5 nanoﬁbers.
2.2. Preparation of V2O5/CNTs Hybrid Film Electrodes
Here, 20 mg of V2O5 and 15 mg of CNTs (length: 0.5–1.5 µm; diameter ~5 nm; Carbon Solutions Inc., Riverside, CA, USA) were dissolved in 40 mL of DMF; then, the mixture was sonicated to form a mixed suspension. The V2O5/CNTs ﬁlm was fabricated by ﬁltration and then dried in an oven at 80 ◦C.
2.3. Material Characterizations Scanning electron microscopy (SEM, Supra-55, Zeiss, Oberkochen, Germany) and transmission electron microscopy (TEM, JEOL2100F, JEOL, Tokyo, Japan) were used to in- vestigate the morphology of the samples. The chemical components of the V2O5/CNTs ﬁlm were conﬁrmed with X-ray photoelectron spectroscopy (XPS, PHI 1600 ESCA, PerkinElmer, Waltham, MA, USA). The structure of the V2O5 nanowires and V2O5/CNTs ﬁlm was char- acterized using X-ray diffraction (XRD, Rigaku D/Max-3A, Rigaku Corporation, Tokyo, Japan). Raman spectra were recorded by a spectrophotometer (Thermo-Fisher Scientiﬁc, Waltham, MA, USA).
2.4. Electrochemical Measurements Stainless-steel CR2032 coin cells were assembled and tested to evaluate the electro- chemical performance of the samples. The cells were assembled using a V2O5/CNTs composite ﬁlm as the cathode, ﬁlter paper as the separator, Zn foil as the anode, and 3 M of aqueous Zn(CF3SO3)2 solution as the electrolyte. Electrochemical impedance spectroscopy (EIS) was performed using a frequency range between 10 mHz and 100 kHz with an AC perturbation signal of 10 mV. Cyclic voltammetry (CV) of the as-assembled battery was conducted at various scan rates (0.2–1.0 mV·s−1). A CHI 660E electrochemical workstation (Shanghai Chenhua, Shanghai, China) was employed to record the CV and EIS results. A CT2001A LAND electrochemical workstation was used to perform the galvanostatic intermittent titration technique (GITT), galvanostatic charge/discharge (GCD), and cyclic Nanomaterials 2021, 11, x FOR PEER REVIEW 3 of 10
Nanomaterials 2021, 11, 1054 3 of 10 CT2001A LAND electrochemical workstation was used to perform the galvanostatic in- termittent titration technique (GITT), galvanostatic charge/discharge (GCD), and cyclic performance, within a voltage window of 0.3–1.5 V. All speciﬁcspecific capacities reported in this work are based on the cathode mass.
The morphology of the as-prepared V2O5 waswas investigated investigated with with a a transmission transmission elec- elec- tron microscopemicroscope (TEM)(TEM) and and scanning scanning electron electron microscope microscope (SEM). (SEM). The The TEM TEM and and SEM SEM images im- agesreveal reveal that the that V2 theO5 hadV2O a5 nanoﬁberhad a nanofiber morphology morphology with a diameter with a diameter of ~18 nm of and ~18 lengths nm and of lengthsseveral micrometersof several micrometers (Figure1a,b). (Figure After 1a being,b). After mixed being with mixed CNTs, thewith V CNTs,2O5 nanoﬁbers the V2O5 werenan- ofibersembedded were into embedded the network into of CNTsthe network (Figure1 c).of Furthermore,CNTs (Figure the 1c). V 2O Furthermore,5/CNTs electrode the Vshowed2O5/CNTs a freestanding electrode showed structure a freestanding (inset of Figure struct1c).ure Elemental (inset of mappings Figure 1c). conﬁrmed Elemental that map- C, pingsO, and confirmed V elements that were C, evenly O, and distributed V elements in thewere V 2evenlyO5/CNTs distributed nanobelts in (Figure the V12Od5)./CNTs XRD nanobeltsand Raman (Figure spectroscopy 1d). XRD tests and were Raman further spectros performedcopy tests to investigate were further the Vperformed2O5 nanoﬁbers to in- and V O /CNTs ﬁlm. XRD patterns of the V O nanoﬁbers and V O /CNTs ﬁlm presented vestigate2 5 the V2O5 nanofibers and V2O5/CNTs2 5 film. XRD patterns2 of5 the V2O5 nanofibers typical (001) and (003) peaks (Figure2a), which ﬁtted well with the layered V O (JCPDS and V2O5/CNTs film presented typical (001) and (003) peaks (Figure 2a), which2 fitted5 well no. 40–1296). Peaks of V O were also detected, which may be ascribed to the reduction with the layered V2O5 (JCPDS4 7 no. 40–1296). Peaks of V4O7 were also detected, which may of V O by P123 . The Raman spectrum of V O /CNTs showed the presence of D be ascribed2 5 to the reduction of V2O5 by P123 .2 The5 Raman spectrum of V2O5/CNTs and G peaks as compared to that of V2O5, indicating the presence of CNTs in composite showed the presence of D and G peaks as compared to that of V2O5, indicating the pres- ﬁlms . The three peaks located at 139, 280, and 983 cm−1 are assigned to the V-O ence of CNTs in composite films . The three peaks located at 139, 280, and 983 cm−1 are vibration in both the V2O5/CNTs and V2O5 samples (Figure2b) [ 20]. In addition, in the assigned to the V-O vibration in both the V2O5/CNTs and V2O5 samples (Figure 2b) . XPS survey spectrum, solely C, V, and O elements were detected, conﬁrming the purity In addition, in the XPS survey spectrum, solely C, V, and O elements were detected, con- of the as-prepared V2O5/CNTs sample (Figure2c). The peak located at 517.5 eV in the V firming the purity of the as-prepared V2O5/CNTs sample (Figure 2c). The peak located5+ at 2p1/2 spectrum and the peak at 525.2 eV in the V 2p3/2 spectrum correspond to V , and 517.5 eV in the V 2p1/2 spectrum and the peak at 525.2 eV in the V 2p3/2 spectrum corre- the peak located5+ at 516.8 eV in the V 2p1/2 spectrum and the peak at 523.7 eV is related spond4+ to V , and the peak located at 516.8 eV in the V 2p1/2 spectrum and the peak at 523.7 to V (Figure2d) [ 18]. The surface area of V2O5/CNTs hybrid ﬁlms was measured to be eV is related to V4+ (Figure 2d) . The surface area of V2O5/CNTs hybrid films was meas- 107 m2 g−1, as shown in Figure2e. ured to be 107 m2 g−1, as shown in Figure 2e.
Figure 1. ((aa)) TEM TEM image image of of the the V V2O25O nanofibers.5 nanoﬁbers. (b) (SEMb) SEM image image of V of2O V5 nanofibers.2O5 nanoﬁbers. (c) SEM (c) image SEM image and optical and optical image image(inset) (inset)of V2O of5/CNTs V2O5 films./CNTs (d ﬁlms.) Element (d) Element mappings mappings of V2O5/CNTs. of V2O 5/CNTs.
Nanomaterials 2021, 11, 1054 4 of 10 Nanomaterials 2021, 11, x FOR PEER REVIEW 4 of 10 Nanomaterials 2021, 11, x FOR PEER REVIEW 4 of 10
FigureFigureFigure 2. 2.2. ( (a(a)a)) XRD XRDXRD patterns patternspatterns of ofof V V2VO22O5 55and andand V V2O2O55/CNTs./CNTs. ( (b)) RamanRaman spectraspectra ofof thethethe V VV22O2O5 5and and V V2O2OO55/CNTs.5/CNTs. ( c( )cc ))XPS XPS spectra spectraspectra of ofof VVV22O2O5/CNTs5/CNTs and and (( dd)) VV 2p2p spectrum.spectrum. spectrum. (( (ee)) Nitrogen Nitrogen adsorption/desorption adsorption/desorption isotherms.isotherms. isotherms.
TheThe electrochemicalelectrochemical propertiesproperties of ofof V VV222OO55 and andand V VV22O2O55/CNTs5/CNTs films films ﬁlms were were further further evaluated evaluated inin ZIBs.ZIBs.ZIBs. TheThe speciﬁcspecific capacitycapacity atatat differentdifferentdifferent current currentcurrent densitiesdensities densities ofof of VV V22O2O5 5andand and VV V22O2OO5/CNTs55/CNTs/CNTs sam- sam- − −11 plesples areare shownshown inin FigureFigure3 a.3a. The TheThe V VV22O2OO555/CNTs/CNTs film ﬁlmfilm showed showedshowed a aa high highhigh capacity capacity of of 399 399 mAh mAh g −g1 −1 −1 −1 −1 atat 0.10.1 AA g−1, ,which which is is higherhigher higher thanthan than thatthat that ofof of thethe the VV2 V2OO25O5 nanofiber nanofiber5 nanoﬁber (312 (312 (312 mAh mAh mAh g g−1). g). The The). Thereason reason reason for for forthethe thecapacitycapacity capacity decreasing decreasing atat lowlow at current lowcurrent current densitiesdensities densities is is ascribed ascribed is ascribed to to the the tocontinuous continuous the continuous V V2O2O5 disso-5 disso- V2O5 −1 dissolutionlutionlution .. Even . Evenat a high at a currentcurrent high current densitydensity density ofof 55 AA ofg g−1− 5,1 ,the Athe g V V2O2,O the5/CNTs5/CNTs V2O film 5film/CNTs still still exhibited ﬁlm exhibited still ex-a a −1 hibitedhighhigh discharge a high dischargecapacity of capacity 239239 mAhmAh of g 239g−−11,, while mAhwhile thegthe , VV while2O2O5 5nanofiber nanofiber the V2O showed 5showednanoﬁber a acapacity capacity showed of of a −1 capacity of− 1871 mAh g . The result demonstrates that the V O /CNTs ﬁlm showed a 187187 mAh g−1. The result demonstratesdemonstrates thatthat thethe VV2O2O5/CNTs5/CNTs film film 2showed showed5 a ahigher higher rate rate ca- ca- higher rate capability than that of V O nanoﬁbers electrode due to the introduction of pabilitypability than that of V22O55 nanofibersnanofibers electrode2electrode5 due due to to the the introduction introduction of of CNTs. CNTs. Figure Figure 3b 3b CNTs. Figure3b displays the charge/discharge curves of the V O /CNTs ﬁlm under vari- displaysdisplays the charge/discharge curvescurves ofof thethe V V22OO55/CNTs/CNTs film film under under2 5 various various current current densi- densi- ousties.ties. current TheThe charge/discharge densities. The curves charge/dischargecurves atat differendifferentt current curvescurrent atdensities densities different showed showed current similar similar densities shapes, shapes, showed in- in- similar shapes, indicating the fast charge transfer kinetics of the V O /CNTs ﬁlm. dicatingdicating the fast charge transfer kineticskinetics ofof thethe V V2O2O5/CNTs5/CNTs film. film. 2 5
FigureFigure 3. 3.( a(a)) The The rate rate performance performance of of the the V 2VO2O5/CNTs5/CNTs ﬁlmfilm andand VV22OO55 electrodes. ( (bb)) Charge/discharge Charge/discharge curves curves of of the the Figure 3. (a) The rate performance of the V2O5/CNTs film and V2O5 electrodes. (b) Charge/discharge curves of the VV2O2O55/CNTs/CNTs ﬁlmfilm andand VV22O5 electrodeselectrodes at at different current densities. ( c) Cycle performanceperformance of VV22O5/CNTs/CNTs film ﬁlm and and V V22OO5 5 V2O5/CNTs film and V2O5 electrodes at different current densities. (c) Cycle performance of V2O5/CNTs film and V2O5 electrodes.electrodes. (d(d)) Long-term Long-term cyclingcycling performanceperformance ofof VV2OO5/CNTs film ﬁlm and V 2OO5 electrodeselectrodes at at 5 5 A A g −−1.1 .((e)e )Nyquist Nyquist plots plots of of electrodes. (d) Long-term cycling performance of V22O55/CNTs film and V22O5 electrodes at 5 A g−1. (e) Nyquist plots of V2O5/CNTs film and V2O5 electrodes. VV22O5/CNTs film ﬁlm and and V V22OO5 5electrodes.electrodes.
Nanomaterials 2021, 11, 1054 5 of 10
−1 In addition, V2O5/CNTs ﬁlms maintain a high discharge capacity of 273 mAh g −1 after 100 cycles at 1 A g (Figure3c). Apart from the good rate capability, the V 2O5/CNTs ﬁlm also displayed an excellent long-term cyclic stability. Even at 5 A g−1 over 2000 cycles, −1 the batteries based on the V2O5/CNTs ﬁlm maintained a capacity of 251 mAh g with a high-capacity retention of 94% (Figure3d), which is much higher than those of pris- −1 tine V2O5 (168 mAh g and 81%). The long cycle capability of the V2O5/CNTs ﬁlm was comparable or higher than most of the previously reported V-based materials with- out CNTs (Table1)[21–31] . Furthermore, compared with other works using CNTs in an V2O5 electrode, the batteries based on the V2O5/CNTs ﬁlm still displayed a comparable capacity and cycle performance (Table2)[ 32–34]. These superior electrochemical perfor- mances could be ascribed to the nanowire V2O5 knitted with CNTs being helpful for the electrode to keep the close contact and provide an effective electron transmission. The electrochemical impedance spectra (EIS) measurements were performed to study the ki- netics. As shown in Figure3e, both the Nyquist plots of the V 2O5 and V2O5/CNTs ﬁlm consisted of a hemicycle at the high-frequency region (charge transfer-limited process) and a straight line in the low-frequency region (ion diffusion-limited process). As for the V2O5/CNTs sample, the line in the low-frequency region was substantially steeper and the inner diameter of the hemicycle in the high-frequency region was small com- pared with V2O5, manifesting that it had a fast ion diffusion rate and a small resistance. The charge transfer resistance (Rct) of the V2O5/CNTs ﬁlm electrode was about 462 Ω after ﬁtting, which is smaller than that of V2O5 (741 Ω), revealing that the introduction of CNTs is beneﬁcial for the high electronic conductivity and efﬁcient Zn2+ transport in the V2O5/CNTs cathode. Furthermore, the energy/power densities were calculated and compared with other cathode materials (Figure4 ). Impressively, the batteries based on the V2O5/CNTs ﬁlm display a remarkable energy density and an impressive power density (e.g., 267 Wh kg−1 and 3.2 kW kg−1), which is comparable with the cathodes of K2V6O16·2.7H2O, VS2, Zn0.25V2O5·nH2O, LiV3O8, Na0.33V2O5, Zn3[Fe(CN)6]2, and Na3V2(PO4)3 [27,30,35–39].
Table 1. The comparison of long-term cycle performances of the V2O5/CNTs cathode.
Rate Final Capacity Cathodes Capacity Retention Reference (A g−1) (mAh g−1)
V2O5/CNTs 5 94% (2000 cycles) 251 This work V2O5·nH2O 6 71.0% (900 cycles) 213  2+ Cu -V2O5 10 88.0% (5000 cycles) 180  + K -V2O5 8 96.0% (1500 cycles) 172  Graphene/H2V3O8 6 87.0% (2000 cycles) 240  V2O5@PANI 5 93.8% (1000 cycles) 201  2D V2O5 20 68.2% (500 cycles) 117  Zn0.25V2O5·nH2O 2.4 80.0% (1000 cycles) 208  NaV3O8·1.5H2O 4 82.0% (1000 cycles) 120  Na2V6O16·3H2O 14 85% (1000 cycles) 129  K2V6O16·2.7H2O 5 88% (229 cycles) 139  Na1.1V3O7.9/rGO 1 93% (500 cycles) 85 
Table 2. The comparison of the V2O5/CNTs cathode with other CNT-based V2O5 electrodes.
Cathodes Speciﬁc Capacity Capacity Retention Reference 399 mAh g−1 (0.1 A g−1) 5A g−1: V O /CNTs This work 2 5 327 mAh g−1 (1 A g−1) 94% (2000 cycles) 10A g−1: V O /CNTs nanopaper 375 mAh g−1 (0.5 A g−1)  2 5 80.0% (500 cycles) 1 A g−1: V O /CNTs (VCP) 312 mAh g−1 (1 A g−1)  2 5 81% (2000 cycles) 5 A g−1: V O @CNTs 293 mAh g−1 (0.3 A g−1)  2 5 72.0% (6000 cycles) Nanomaterials 2021, 11, x FOR PEER REVIEW 6 of 10
1 A g−1: V2O5/CNTs (VCP) 312 mAh g−1 (1 A g−1)  81% (2000 cycles) Nanomaterials 2021, 11, 1054 6 of 10 5 A g−1: V2O5@CNTs 293 mAh g−1 (0.3 A g−1)  72.0% (6000 cycles)
Figure 4. Ragone plot of the batteries based on V2O5/CNTs compared with oher reported data for Figure 4. Ragone plot of the batteries based on V2O5/CNTs compared with oher reported data forZIBs. ZIBs.
TheThe electrochemical electrochemical kinetics kinetics was was further further investigated investigated to to explain explain the the electrochemical electrochemical performance.performance. The The CV CV curves curves of of the the V2 VO25O/CNTs5/CNTs ﬁlm film was was measured measured at at different different scan scan rates. rates. AsAs shown shown in in Figure Figure5a, 5a, the the CV CV curves curves showedshowed similarsimilar shapes with with the the growth growth of of the the scan scanrates, rates, which which indicates indicates its itsgood good electrochemical electrochemical reversibility. reversibility. The The characteristic characteristic peaks peaks ap- appearedpeared at at 0.5/0.7 0.5/0.7 V, V, as as well well as as0.8/1.0 0.8/1.0 V, reflecting V, reﬂecting the theredox redox reaction reaction in V in2O5 V/CNTs2O5/CNTs (Figure (Figure5a) [15,18].5a) [ 15 According,18]. According to the to previous the previous literature, literature, the thepeak peak current current (i) (i)and and scan scan rates rates (v) (v)have have a alinear linear relationship, relationship, which which can can be be written written as as : :